Advisory Note Distortion becoming a diminishing event GEN/13/1 June 2001 There is a perception that distortion of fabricated steel items is a significant problem, however, is reality, distortion occurs in only a very small number of instances. Distortion has become a rare occurrence as bath sizes and handling facilities have improved. Over recent years the after fabrication galvanizing industry has undergone major upgrades in terms of steel handling capabilities and larger plant capacity which has resulted in a further reduced incidence of distortion occurring when fabricated steel articles are galvanized. Occurrence Galvanizing will not generally cause distortion provided that design and fabrication principles are correct. When steel fabrications do distort during galvanizing, the reasons have usually been ‘built-in’ at an earlier stage. Distortion almost always arises from the relief of stresses as the steel is heated to the galvanizing temperature (usually 445- 465OC). Although such stresses may be inherent in the steel and may vary from batch to batch, they are more commonly caused during fabrication. Distortion may also occur if steels of significantly different thicknesses are joined together in a fabrication. Only very rarely is it caused by handling in the galvanizing plant. Basic design points and other means of minimising distortion are outlined in this leaflet. Symmetrical section (l - beams, tubes), have less inherent tendency to distort than asymmetrically ones (channels). Similarly, cylindrical vessels are less liable to distort than rectangular or elliptical ones. Other things being equal, the lighter the gauge of steel, the greater the risk of distortion. Designer, fabricator and galvanizer should pool their knowledge at an early stage to get best results. Inherent Stresses In Steel Steel invariably contains internal stresses, hot dip galvanizing can release or vary the amount of stress, making distortion possible. Fabrication Stresses Minimising introduction of stresses during welding. Welding results in extreme differences in temperatures within small areas of an assembly and hence in significant residual stresses. In general it is recommended that: • Components of an assembly should be preformed accurately so that they need not be forced, sprung or restrained during welding. • Thick sections should be continuously welded, thin sections and sheet fabrications may benefit from intermittent welding, depending on whether or not heat is conducted rapidly away from the weld, although more stress may arise at the starting point of the weld. • As far as possible, welded assemblies should be aligned so that the stresses are balanced rather than all pulling in the same direction. Other design features to avoid or minimise distortion Steel sections should vary as little as possible. Thick and thin sections absorb and lose heat at different rates and so can expand and contract unevenly. Large unsupported flat sheets may tend to buckle so stiffeners should be included in the design. Frames around the flat panel, whether of solid steel or open material such as welded mesh should be galvanized separately, as the frame would offer a constraint and so tend to cause buckling rather than reduce it. Where there is an inherent tendency to distort e.g. in asymmetrically shaped fabrications (including fabricated girders or lattice beams with top or bottom chords of different sections), the effect can be minimised or possibly eliminated if the fabrications is of such a size and design that it can be rapidly immersed in a single dip. Whether or not this can be done will depend on both the size of the sections in relationship to the galvanizer’s dipping facilities, and also on the extent to which hollow sections are involved. The galvanizer should be consulted to decide on the maximum advisable lengths. There is little or no distortion in standard symmetrical components whether they are single or double- end dipped - however if larger fabrications need to be double- end dipped, the significant thermal gradient created by this procedure may give rise to distortion. Where some bowing, twisting or bending has occurred it may be possible to straighten the object after the galvanizing process. Stress Relief Fabrication stresses can sometimes be eliminated by stress relieving before galvanizing. Early consultation between galvanizer, fabricator and designer is the key to success in avoiding distortion, through the incorporation of good design features. Basic design considerations are shown on the reverse side of this leaflet. Plate Products Plate material can present a distortion risk, especially plate under 10 mm in thickness. To minimise distortion problems, the following rules should be observed: • Where possible, galvanize the plate separately from any frame or supporting steel work and assemble after galvanizing • Recommend that uniform processing of the plate be specified during fabrication; i.e. Shear the plate where possible and minimise oxy cutting of long edges • Putting holes in the centre of floor plates will assist in minimising buckling as the plate expands into the hole during heating • Specify air cooling where possible • Avoid double dipping where possible This Advisory Note is intended to keep readers abreast of current issues and developments in the field of galvanizing. The Galvanizers Association of Australia has made every effort to ensure that the information provided is accurate, however its accuracy, reliability or completeness is not guaranteed. Any advice given, information provided or procedures recommended by GAA represent its best solutions based on its information and research, however may be based on assumptions which while reasonable, may not be applicable to all environments and potential fields of application. Due and proper consideration has been given to all information provided but no warranty is made regarding the accuracy or reliability of either the information contained in this publication or any specific recommendation made to the recipient. Comments made are of a general nature only and are not intended to be relied upon or to be used as a substitute for professional advice. GAA and its employees disclaim all liability and responsibility for any direct or indirect loss or damage which may be suffered by the recipient through relying on anything contained or omitted in this publication. So long as no alterations are made unless approved, you are invited to reproduce the information contained in this advice provided acknowledgement is given that GAA is the source.